Semiconductor nanowires have opened new research avenues in quantum transport owing to their confined geometry and electrostatic tunability. They have offered an exceptional testbed for superconductivity, leading to the realization of hybrid systems combining the macroscopic quantum properties of superconductors with the possibility to control charges down to a single electron. These advances brought semiconductor nanowires to the forefront of efforts to realize topological superconductivity and Majorana modes. A prime challenge to benefit from the topological properties of Majoranas is to reduce the disorder in hybrid nanowire devices. Here we show ballistic superconductivity in InSb semiconductor nanowires. Our structural and chemical analyses demonstrate a high-quality interface between the nanowire and a NbTiN superconductor that enables ballistic transport. This is manifested by a quantized conductance for normal carriers, a strongly enhanced conductance for Andreev-reflecting carriers, and an induced hard gap with a significantly reduced density of states. These results pave the way for disorder-free Majorana devices.
Majorana modes are zero-energy quasiparticles emerging at the boundary of a topological superconductor1,2,3. Following proposals for their detection in a semiconductor nanowire coupled to a superconductor4,5, several electron transport experiments reported characteristic Majorana signatures6,7,8,9,10,11,12,13,14. The prime challenge to strengthen these signatures and unravel the predicted topological properties of Majoranas is to reduce the remaining disorder in this hybrid system. Disorder can mimic zero-energy signatures of Majoranas15,16,17,18,19, and results in states within the induced superconducting energy gap20, the so-called soft gap, which renders the topological properties experimentally inaccessible21,22. The soft gap problem is attributed to the inhomogeneity of the hybrid interface20,23,24,25 and has been overcome by a recent demonstration of epitaxial growth of Al superconductor on InAs nanowires23, yielding a hard gap—a strongly reduced density of states within the induced superconducting gap. However, the Al-InAs nanowire system still contains residual disorder showing up in transport as unintentional quantum dots13,23, a common observation in many previous instances of hybrid nanowire devices9,18,19. As an alternative material system, we have further developed the combination of InSb nanowires with NbTiN as our preferred choice of superconductor6. InSb is in general cleaner (that is, higher electron mobility26,27,28,29) than InAs. Moreover, InSb has a ∼5 times larger g-factor, bringing down the required external magnetic field needed to induce the topological phase transition. Our preference for NbTiN relies on its high critical magnetic field exceeding 10 T.
Here we show ballistic superconductivity in InSb semiconductor nanowires. Our structural and chemical analyses demonstrate a high-quality interface between the InSb nanowire and a NbTiN superconductor. The high-quality interface enables ballistic transport manifested by a quantized conductance for normal carriers, and a strongly enhanced conductance for Andreev-reflecting carriers at energies below the superconducting gap. Our numerical analysis indicates a mean free path of several micrometres, implying ballistic transport of Andreev pairs in the proximitized nanowire. Finally, tunnelling conductance reveals an induced hard gap with a significantly reduced density of states. These results constitute a substantial improvement in induced superconductivity in semiconductor nanowires, and pave the way for disorder-free Majorana devices.
Hybrid nanowire devices and their structural analysis
We report on five devices with different geometries all showing consistent results. An overview of all the devices is given in Supplementary Fig. 1. Figure 1a,b shows a nanowire device consisting of a normal contact (Au), a nanowire (InSb) and a superconducting contact (NbTiN). This device was first measured at low temperature showing high-quality electron transport (data discussed below). After, the device was sliced open (using focused ion beam) and inspected sideways in a transmission electron microscope (TEM). The hexagonal facet structure of the nanowire is clearly visible (Fig. 1c and Supplementary Fig. 2). Except for the bottom facet that rests on the substrate, the polycrystalline superconductor covers the nanowire all around without any visible voids.
The precise procedure for contact realization is extremely important (see ref. 25). First, the native oxide at the InSb surface is wet-etched using a sulfur-based solution followed by an argon etch of sufficiently low power to avoid damaging the InSb surface (see Methods). The inclusion of sulfur at the interface results in band bending with electron accumulation near the surface of InSb30 (Supplementary Fig. 3). Superconducting film deposition starts with NbTi, a reactive metal whose inclusion as a wetting layer is crucial to create a good electrical contact. Figure 1d shows that our cleaning procedure only minimally etches the wire and the InSb crystalline properties are preserved after the deposition (details in Supplementary Fig. 2). We detect a thin segregation layer (∼2 nm) between the polycrystalline NbTi and single-crystalline InSb. The chemical analysis (Fig. 1e,f) shows a material composition in agreement with our deposition procedure. More importantly, the inclusion of sulfur is clearly visible at the interface whereas the original native oxide is completely absent.
The high-quality structural properties in Fig. 1 result in largely improved electronic properties over the previous instances of hybrid nanowire devices. Figure 2a shows the differential conductance dI/dV while varying the bias voltage V between the normal and superconducting contacts, and stepping the gate voltage Vgate applied to the global back gate (Fig. 1b). We first of all note that throughout the entire gate voltage range in Fig. 2 we do not observe signs of the formation of unintentional quantum dots or any other localization effects resulting from potential fluctuations. Instead, we observe conductance plateaus at 2e2/h for all devices, typical for ballistic transport and a clear signature of disorder-free devices. For a sufficiently negative gate voltage the non-covered nanowire section between normal and superconducting contacts is depleted and serves as a tunnel barrier. A vertical line cut from this regime is plotted in Fig. 2b, showing a trace typical for an induced superconducting gap with a strong conductance suppression for small V. The extracted gap value is Δ*=0.8 meV. Increasing Vgate first lowers and then removes the tunnel barrier completely. A vertical line cut from this open regime is plotted in Fig. 2c. In this case, the conductance for small V is enhanced compared to the value above ∼1 mV. Note that the range in V showing an enhanced conductance in Fig. 2c corresponds to the same range showing the induced gap in Fig. 2b. The enhancement results from Andreev processes where an incoming electron reflects as a hole at the normal conductor-superconductor interface generating a Cooper pair23,24,31,32. This Andreev process effectively doubles the charge being transported from e to 2e enhancing the subgap conductance. In Fig. 2c, the observed enhancement is by a factor ∼1.5.
The Andreev enhancement is also visible in horizontal line cuts as shown in Fig. 2d. The above-gap conductance (black trace) taken for |V|=2 mV represents the conductance for normal carriers, Gn. The subgap conductance, Gs, near V=0 (Fig. 2d, red trace) shows an Andreev enhancement in the plateau region. Figure 2e shows a similar trace from another device where the enhancement in Gs reaches 1.9 × 2e2/h, very close to the theoretical limit: an enhancement factor of 2 in the case of a perfect interface. Finally, we note the dip in subgap conductance Gs following the Andreev enhancement, observed both in Fig. 2d and Fig. 2e. The combined enhancement and dip structure provides a handle for estimating the remaining disorder by a comparison to theory, as discussed below.
We construct a tight binding model of our devices (Fig. 3a) and numerically calculate the conductance using the Kwant package33 (see Methods for details). In Fig. 3b, we plot the conductance traces obtained from the simulation for different disorder strength corresponding to varying mean free paths le. The calculated subgap conductance reproduces the dip structure observed in the experiment. We find that the dip is caused by mixing between the first and the second subband due to residual disorder (Supplementary Fig. 4). Even for weak disorder, subband mixing is strongly enhanced near the opening of the next channel, due to the van Hove singularity at the subband bottom. Hence, the Andreev conductance will generically exhibit a dip close to the next conductance step, instead of a perfect doubling. Figure 3c shows the measured subgap conductance Gs and above-gap conductance Gn for a device with a particularly flat plateau. Comparing Fig. 3b and Fig. 3c, we find good agreement for a mean free path of several micrometres. This implies ballistic transport of Andreev pairs in the proximitized wire section underneath the superconductor, whose length far exceeds the length of the non-covered wire between the contacts (see also Supplementary Fig. 5). Andreev enhancement allows for extracting mean free paths greatly exceeding the non-covered wire section since the subgap conductance is sensitive to even minute disorder in the proximitized wire section—a new finding of our study. This sensitivity is due to the quadratic dependence of the subgap conductance on the transmission probability (introduced below). In Fig. 3d,e, we compare a conductance measurement similar to the one in Fig. 2a with the simulation of a ballistic device. The overall agreement indicates a very low disorder strength for our devices.
Hard superconducting gap
The theory for electronic transport from a normal conductor via a quantum point contact to a superconductor was developed by Beenakker31. The subgap conductance is described by Andreev reflections32, and for a single subband given by . The gate voltage-dependent transmission probability T can be extracted from the measured above-gap conductance, given by . Figure 4a shows excellent agreement between the calculated and measured subgap conductance up to the point where the measured Andreev enhancement is reduced due to subband mixing. The highest transmission probability obtained from Andreev enhancement sets a lower bound on the interface transparency. Our typical enhancement factor of 1.5 (Figs 2d and 3c) implies an interface transparency ∼0.93 and our record value of 1.9 (Fig. 2e) gives a transparency larger than 0.98 (see Measurement setup and data analysis in Methods).
The comparison between Gs versus Gn can be continued into the regime of an increasing tunnel barrier. Figure 4b,c show traces of dI/dV for successively lower conductances. The subgap conductance suppression reaches , a value comparable to the results obtained with epitaxial Al23. A comparison between the measured subgap conductance and Beenakker’s theory (without any fit parameters) is shown in Fig. 4d. The excellent agreement over three orders of magnitude in conductance implies that the subgap conductance is very well described by Andreev processes and no other transport mechanisms are involved23,24. The lowest conductance () reaches our measurement limit, causing the deviation from theory. The inset to Fig. 4b shows how the subgap conductance increases when applying a magnetic field. Finally, in Supplementary Fig. 6 we show the magnetic field dependence of the induced gap and Andreev enhancement for a magnetic field along the nanowire axis. We again find a subgap conductance increasing with magnetic field, and an Andreev enhancement vanishing at a magnetic field (<1 T) smaller than the critical field of our NbTiN film. We speculate that the increasing subgap conductance and the decreasing Andreev enhancement are due to vortex formation in our NbTiN film, a type-II superconductor. Future studies should be directed towards developing a quantitative description of such magnetic field-induced deviation from Andreev transport, whose understanding plays a crucial role in realizing a topological quantum bit based on semiconductor nanowires.
Nanowire growth and device fabrication
InSb nanowires have been grown by Au-catalysed vapour–liquid–solid mechanism in a metal organic vapour phase epitaxy reactor. The InSb nanowire crystal direction is  zinc blende, free of stacking faults and dislocations34. Nanowires are deposited one-by-one using a micro-manipulator35 on a substrate covered with 285 nm thick SiO2 serving as a gate dielectric for back-gated devices. For local-gated device D, extra set of bottom gates are patterned on the substrate followed by transfer of h-BN (∼30 nm thick) onto which nanowires are deposited. The contact deposition process starts with resist development followed by oxygen plasma cleaning. Then, the chip is immersed in a sulfur-rich ammonium sulfide solution diluted by water (with a ratio of 1:200) at 60 °C for half an hour36. At all stages care is taken to expose the solution to air as little as possible. For normal metal contacts27, the chip is placed into an evaporator. A 30 s Helium ion milling is performed in situ before evaporation of Cr/Au (10 nm/125 nm) at a base pressure <10−7 mbar. For superconducting contacts25, the chip is mounted in a sputtering system. After 5 s of in situ Ar plasma etching at a power of 25 W and an Ar pressure of 10 mTorr, 5 nm NbTi is sputtered followed by 85 nm NbTiN.
Measurement setup and data analysis
All the data in this article is measured in a dilution refrigerator with a base temperature of around 50 mK using several stages of filtering. The determination of the Andreev enhancement factor depends sensitively on the contact resistance subtracted from the measured data. In all our analysis, we only subtract a fixed-value series resistance of 0.5 kΩ solely to account for the contact resistance of the normal metal lead. This value is smaller than the lowest contact resistance we have ever obtained for InSb nanowire devices27, which makes the values for the interface transparency a lower bound.
The cross-section and lamella for TEM investigations were prepared by focused ion beam (FIB). FIB milling was carried out with a FEI Nova Nanolab 600i Dualbeam with a Ga ion beam following the standard procedure37. We used electron induced Co and Pt deposition for protecting the region of interest and a final milling step at 5 kV to limit damage to the lamella. High-resolution TEM (HRTEM) and scanning TEM analyses were conducted using a JEM ARM200F aberration-corrected TEM operated at 200 kV. For the chemical analysis, energy-dispersive X-ray measurements were carried out using the same microscope equipped with a 100 mm2 energy-dispersive X-ray silicon drift detector (SSD).
Characterization of NbTiN
Our NbTiN films are deposited using an ultrahigh vacuum AJA International ATC 1800 sputtering system (base pressure ∼10−9 Torr). We used a Nb0.7Ti0.3 wt.% target with a diameter of 3 inches. Reactive sputtering resulting in nitridized NbTiN films was performed in an Ar/N2 process gas with 8.3 at.% N2 content at a pressure of 2.5 mTorr using a DC magnetron sputter source at a power of 250 W. An independent characterization of the NbTiN films gave a critical temperature of 13.3 K for 90 nm thick films with a resistivity of 126 μΩ· cm and a compressive stress on Si substrate.
Details of the theoretical simulation
The system is described by the spin-diagonal Bogoliubov–de Gennes Hamiltonian
acting on the spinor . The Pauli matrices act on the electron-hole degree of freedom. Potential in the nanowire is described by , where describes a quantum point contact given by
Here YQPC is the centre position of the barrier (Fig. 3a). Barrier width is W=60 nm, and the barrier height is controlled by VQPC. The softness of the barrier is given by λ which we take 5 nm. VD(x, y, z) accounts for disorder, which is modelled as a spatially varying potential with random values from a uniform distribution within a range [−U0, U0] where amplitude is set by mean free path le.
We approximate the superconductor covering the wire by a layer of non-zero Δ for and y>LN and z>−R. The huge wave vector difference in the superconductor and semiconductor cannot be captured in a numerical simulation of a three-dimensional device. Hence, to capture the short coherence length in the superconductor, we take a superconducting shell of thickness RS=10 nm and Δ=200 meV. We then tune the induced gap to be close to the experimental value (∼0.5 meV) by reducing the hopping between the semiconductor and the superconductor by a factor of 0.8.
The transport properties of the system are calculated using Kwant package33 with the Hamiltonian in equation (1) discretized on a three-dimensional mesh with spacing a=7 nm and infinite input (normal) and output (normal/superconducting) leads. For a given VOPC and excitation energy ɛ we obtain the scattering matrix of the system from which we subsequently extract electron re(ɛ) and hole rh(ɛ) reflection submatrices. Finally, we calculate thermally averaged conductance for injection energy E=−eV according to
where the Fermi function
and . We assume chemical potential to be μ=30 meV, which gives N=3 spin-degenerate modes in the leads. The presented results are obtained for T=70 mK and InSb effective mass m*=0.014me.
All data are available at http://doi.org/10.4121/uuid:fdeb81ab-1478-4682-9f48-dec1c83242bd (ref. 38). The code used for the simulations is available upon request.
How to cite this article: Zhang, H. et al. Ballistic superconductivity in semiconductor nanowires. Nat. Commun. 8, 16025 doi: 10.1038/ncomms16025 (2017).
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
We thank A.R. Akhmerov, O.W.B. Benningshof, A. Geresdi, J. Kammhuber and A.J. Storm for discussions and assistance. This work has been supported by the Netherlands Organisation for Scientific Research (NWO), Foundation for Fundamental Research on Matter (FOM), European Research Council (ERC) and Microsoft Corporation Station Q.
About this article